2.2.2. Injection Molding

Testing samples were molded using an injection molding machine Ergotech 110– 430h/310V from DEMAG (Demag, Germany). The injection conditions used to develop recycled TPS and biocomposite TPS/AASP test specimens are listed in Table 4. After each injection cycle, the material was milled and dried at 60 ◦C for 6 h. Then, TPS was processed a total of four cycles and TPS/ASP biocomposite six cycles. The difference in the number of processing cycles between TPS and TPS/ASP was due to the poor quality of the specimens after TPS-4. TPS-5 presented injection defects, such as shrinkage. The nomenclature of recycled TPS and TPS/ASP biocomposite is given in Table 5. Specimens were conditioned at a temperature of 23 ◦C and relative humidity of 50% for at least 16 h before testing.

**Table 4.** Injection condition of starch-based polymer and biocomposite.



**Table 5.** Nomenclature of recycled biocomposite.
